BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS


 Patrick Perkins
 1 years ago
 Views:
Transcription
1 BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency , Ohsawa, Mitaka, Tokyo, JAPAN ABSTRACT In this study, biaxial failure strength of quasiisotropic CFRP (carbon fiber reinforced plastic) composite laminate was investigated experimentally. Inplane biaxial tests with using CFRP cruciform specimens were conducted to measure biaxial failure strains with strain gauges. High speed photographs of biaxial fracture indicated that failure in the cruciform specimen was initiated at gauge area and breakage was developed to GFRP (glass fiber reinforced plastic) tab regions of the specimen. Failure strains under uniaxial stress measured with the cruciform specimens were compared with those measured with strip specimens. Both failure strains were approximately coincident, which proved the validity of the inplane biaxial strength tests with cruciform specimens. Failure strain in the direction of higher load was approximately constant in the first quadrant of failure envelope. Failure strain under uniaxial tensile stress was higher than those under biaxial tensile stress. Keywords: CFRP laminate, Biaxial load, Cruciform Specimen, Failure Envelope, Biaxial Strength INTRODUCTION New engineering materials are being developed to improve performance for vehicle structures. Especially, light weight and high strength materials are expected in aeronautical, astronautical and transportation industries. Applications of composite materials, as light weight materials, are recently widening for aerospace structures. Multiaxial failure criteria of the composite materials are very important for design of the aerospace structures, but have been not yet sufficiently established due to microscopic anisotropy and complicated fracture mechanisms in the composite materials. Many damage and failure criteria for composite materials under multiaxial stresses have been proposed and evaluated using experimental data [1]. Substantial experimental data is needed to assess the prediction by the proposed criteria. However, multiaxial strength data is not enough for new materials because multiaxial testing methods do not become widely used due to difficulties to conduct tests and particularity of facilities. Many methods to evaluate the multiaxial mechanical characteristics are suggested. One of the effective methods to acquire the biaxial mechanical properties of the plate is an inplane biaxial testing with a planar cruciform specimen.
2 Inplane biaxial tests with cruciform specimens had been employed to measure the biaxial mechanical properties of fabrics and yield locus of metal materials for decades. Recently biaxial mechanical properties of composite materials were obtained with using cruciform specimens. Mailly et al.[2] measured biaxial strength of GFRP unidirectional materials with cruciform specimens. They reported substantial influence of longitudinal stress on transverse nonlinearity of GFRP materials. Smits et al.[3] investigated effect of cruciform specimen geometries on biaxial failure strain of GFRP laminates, and determined a suitable geometry for biaxial testing of fiber reinforced composites. Welsh et al.[4] experimentally acquired twodimensional failure envelope for quasiisotropic CFRP laminates with using cruciform specimens, and estimated failure stress with φ R φ160 φ [unit:mm] Fig.1. CFRP cruciform specimen. Fig.2. Biaxial Testing Machine. Fig. 3. Finite element mesh of quarter model of cruciform specimen. Table 1. Elastic constants of HTA/#101 CF/epoxy quasiisotropic laminate. Property E(GPa) 49.4 G(GPa) 18.9 ν 0.31 Table 2. Elastic constants of GFRP laminate. Property E(GPa) 30.0 G(GPa) 11.5 ν 0.3
3 bypass correction factor. In Japan Aerospace Exploration Agency(former National Aerospace Laboratory of Japan), Susuki[5] conducted biaxial fatigue tests with cruciform specimens for fiber reinforced composites in addition to static fracture tests, and the results indicated that biaxial loading phase has significant impact on fatigue strength of the composite laminates. Khamsesh et al.[6] carried out openhole biaxial compression tests for CFRP composite laminates, and identified failure mechanisms of composite laminate with openhole under biaxial compressive load. In this study, biaxial strength of quasiisotropic CFRP composite laminates was experimentally acquired. Inplane biaxial tests with using CFRP cruciform specimens were conducted to measure biaxial failure strains with strain gauges. Strain and stress distributions in gauge area of the cruciform specimen were evaluated by finite element analysis and compared to validate measured strain level and ratio. Failure strains under uniaxial stress measured with the cruciform specimens were compared with those measured with strip specimens to prove the validity of the inplane biaxial strength tests. Influence of biaxial loadings on failure strains of quasiisotropic CFRP laminates were evaluated by the experimental results. EXPERIMENTAL PROCEDURE Cruciform Specimen Material used in this study was carbon fiber/180 C cured epoxy HTA/#101. Stacking sequence of specimens was (0/90/45/45)s. Thickness of the laminates was about 1.0mm. GFRP tabs are bonded on both sides of the CFRP laminate. Geometry of the biaxial cruciform specimens is shown in Fig. 1. The cruciform specimen geometry was determined based on specimens that Susuki proposed in [5]. The cruciform specimen was designed to apply the biaxial load with pin connections between four arms of the cruciform specimen and cross heads of a biaxial testing machine. However, applying load to the specimen with the pin connections was insufficient to achieve the final failure. Then hydraulic wedge grips were employed to connect the arms of the cruciform specimen to the cross heads of the biaxial testing machine in this study. InPlane Biaxial Testing Machine The biaxial testing machine used in this study consists of four hydraulic actuators of 245kN (tension/compression) capacity for static load. These four actuatorassemblies are diagonally mounted in an octagonal boxshaped frame (Fig. 2). Each loading axis is depicted as x and yaxis. The testing machine can apply biaxial load with arbitrary load ratio to a cruciform specimen. One advantageous aspect of inplane biaxial tests with cruciform specimens is that biaxial strain or stress ratio can be set arbitrarily. A particular problem with the operation of cruciform type biaxial test has been controlling to minimize the drift of the specimen center with load control. A small rigid movement during the biaxial test can give undesirable side force and unexpected damage to the cruciform specimen. It seems to be difficult to control four actuators not to generate imbalance at all by load feedback signals only. A double loop feedback control system was developed to carry out static tests and fatigue tests without readjustments of the specimen position.
4 Because of the round shaped reinforcement of GFRP tabs around the gauge area, stresses in the center portion of the specimen are not simply predictable. Before biaxial strength tests, the strains induced by the biaxial loads in the gauge area are needed to be obtained as functions of biaxial load. The relationships between biaxial loads and strains are used to determine biaxial load ratio to achieve prescribed biaxial strain (or stress) ratio. FINITE ELEMENT ANALYSIS Strain and stress distributions in the gauge area of the cruciform specimen were evaluated with using ABAQUS 6.71, a commercial software package for finite element analysis developed by SIMULIA. The elastic constants of carbon fiber/180 C cured epoxy HTA/#101 quasiisotropic laminate and GFRP laminate used in the numerical analysis are shown in Tables 1 and 2, respectively. The symbols E, G, ν in these tables refer to extensional modulus, shear modulus and Poisson s ratio, respectively. The calculations for the cruciform specimen under biaxial loadings were conducted under the assumptions of linearelastic and nondamage development with 1/4 model as shown in Fig. 3. The finite element model consists of 8node brick elements. It is assumed for simplicity that there are no holes in the arms of the cruciform specimen and biaxial load was applied to arm ends of the cruciform specimen directly. In this study, x and y axes coincide with the 0º and 90º directions of laminates respectively, and the z axis is the direction through the ply thickness. RESULTS AND DISCUSSIONS Calculated Strain and Stress Distributions Numerically calculated stress and strain distributions in the CFRP cruciform specimen under uniaxial loading F x =100kN, F y =0kN (F x : F y =1:0) are shown in Fig. 4, where F x and F y mean x and ydirectional applied forces, respectively. Xdirectional stress and strain in the gauge area are higher than other regions as shown in Fig. 4(a) and (b), respectively. Ydirectional stress in the gauge area in Fig. 4(c) was compressive when the specimen is subjected to xdirectional uniaxial tensile load. Ratio of ydirectional contraction in Fig. 4(d) to xdirectional extension in Fig. 4(b) is higher than Poisson's ratio due to the transverse compression. It is noted that stress field is not uniaxial stress state in the gauge area of the cruciform specimen, even though the cruciform specimen is subjected to uniaxial load. Calculated stress and stress distributions in the CFRP laminate under biaxial loading F x = F y =100kN (F x : F y =1:1) are shown in Fig. 5. Stress and strain distributions in case of F x = F y are symmetrical about the line x=y because the cruciform specimen geometry, the stacking sequence and the applied biaxial load are symmetric. Biaxial stress and strain ratios in the gauge area are also 1:1 when the specimen is subjected to biaxial load with load ratio F x : F y =1:1. Maximum normal stress and strain in the gauge area in Fig.5(F x : F y =1:1) are less than those in Fig. 4(F x : F y =1:0) due to Poisson s ratio and round shaped reinforcement of GFRP tabs. Numerical and experimental results of biaxial strains under uniaxial and biaxial loading (F x : F y =1:0 and 1:1) in the strain range within 0.3% are compared in Fig. 6. These
5 figures show that numerical results are in good agreement with experimental results, and biaxial strain ratio changes in relation to the biaxial loading ratio. Relationships among Biaxial Load, Strain and Stress Relationships among xdirectional uniaxial load F x, strains (ε x and ε y ) and stresses (σ x and σ y ) in the strain range within 0.3% are shown in Fig. 7, where ε i and σ i (i=x, y) are idirectional normal strain and stress, respectively. Strains (ε x and ε y ) were measured by using strain gauges. Stress in the gauge area can be calculated from cross sectional area in the gauge area and force that carried through the gauge area conceptually. Applied force to the cruciform specimen is carried through not only the gauge area but also other regions of the specimen. However, fraction of the force carried through gauge area is depend on specimen geometry and material constants, and unable to be determined simply. Then, stresses (σ x and σ y ) had to be calculated from elastic constants and the biaxial strains. In Fig. 7, ydirectional stress σ y is negative value, which means that gauge area is transversely compressed even though the specimen is subjected to uniaxial load. Biaxial strains under certain biaxial load ratios can be calculated based on the relationship between biaxial strains and uniaxial load with superposition principle in the y mal Stress x (a) xdirectional stress (Pa) mal Strain (b) xdirectional strain (m/m) E E y mal Stress x (c) ydirectional stress E+81.5E+8 (Pa) (m/m) Fig. 4. Calculated normal stress and strain in cruciform specimens under uniaxial loading (F x =100kN, F y =0kN). mal Strain (d) ydirectional strain
6 y mal Stress x (a) xdirectional stress (Pa) (m/m) Fig. 5. Calculated xdirectional normal stress and strain in cruciform specimens under uniaxial loading (F x =100kN, F y =100kN). range of linear elastic. As an example, several relationships among strain ratio, load ratio and stress ratio are shown in Table 3. In the table, stress is calculated by using strain and elastic constants in Table 1. These ratios are not necessarily coincident with each other with the exception of ratio 1:1 and 1:1. It is noted in the inplane biaxial tests with the cruciform specimens that load ratio has to be determined based on the relationships between load ratio and strain ratio in the gauge area. mal Strain (b) xdirectional strain Failure under Biaxial Loading Relationships between load and strain under biaxial load F x : F y =0.21:1 and 1:1 in the biaxial fracture tests are shown in Fig. 8. In Fig. 8(a), the cruciform specimen was subjected to biaxial load with load ratio F x : F y =0.21:1, and x and ydirectional strains increased as if stress state is uniaxial, which means ratio of xdirectional contraction to ydirectional extension is equal to Poisson s ratio. In Fig. 8(b), x and y directional strains increase accordance with applied load approximately equally due to the load ratio F x : F y =1:1. Inclination of the strain curves after the half of the fracture load are slightly changing in accordance with applied load, though strains at an early stage of the biaxial loading are almost proportional to the applied load. It is supposed that damages such as matrix cracks occurred at the later stage of the fracture tests and the degradation of stiffness due to the damages were the cause of the inclination change at the later stage of the fracture. Photographs of fracture near the gauge area of the cruciform specimen under biaxial loading F x : F y =1:1 were taken by a high speed camera (model:exilim EXF1, Casio Computer Co., Ltd., Japan) as shown in Fig. 9. The photographs were taken with frame rate 300 frame/second and resolution pixels. Figure 9 indicates that fracture was initiated at the gauge area, and subsequently breakage in GFRP tabs was developed in the directions of x and y axes. Photographs of the cruciform specimens after the biaxial fracture tests with load ratio F x : F y =0.21:1 and 1:1 are shown in Fig. 10. Breakage in the cruciform specimen with load control typically reaches the free edge of the cruciform specimens, especially
7 corner fillets. Figure 10 reveals that the breakage stops away from the free edges of the cruciform specimens, though the biaxial load was applied to the specimen with load control. In the experiments, the control system of the biaxial testing machine detects drastic load reduction, which means the stiffness reduction due to the fracture at the gauge area, and immediately activated an emergency stop with displacement control before the breakage reaches the free edges of the specimen. Fractures under ydirectional uniaxial stress at the gauge area was developed to x direction only as shown in Fig.10(a). Fractures under biaxial stress (σx=σy) was developed to both x and ydirections from the gauge area as shown in Fig. 10(b). Effect of Biaxial Loadings on Biaxial Strength Biaxial failure strain measured with using the cruciform specimens is shown in Fig. 11. In this figure, failure strain measured with using strip specimens under uniaxial loading is also plotted. The strip specimen size was 150mm length, 15mm width and 1mm thickness. Stacking sequence of the strip laminate was (45/0/45/90)s. Fracture strains obtained with the strip specimens were approximately equal to those obtained with the cruciform specimens in the uniaxial stress condition. The approximated correspondence of fracture strains under uniaxial stress in both strip and cruciform specimens indicates validity of inplane biaxial strength testing with cruciform specimens. Biaxial failure strains with strain ratios ε x : ε y =1:1, 0.3:1, 0.3:1, and 0.7:1 are plotted in Fig. 11. In the first quadrant of Fig. 11 (ε x : ε y =1:1, 0.3:1), ydirectional failure strains are approximately constant irrespective of xdirectional failure strain. In the second quadrant of Fig. 11(ε x : ε y =0.3:1, 0.7:1), ydirectional failure strains are also approximately constant irrespective of xdirectional failure strain. Comparing the first and second quadrants, ydirectional failure strains in the second quadrant are larger than those in the first quadrant. However, more data for biaxial strength is required to widen the range of failure envelope to all quadrants and to decrease sampling error due to the small samples. CONCLUSIONS The biaxial strength of quasiisotropic CFRP laminates was experimentally acquired with using the cruciform specimens. Strain and stress distributions in gauge area of the cruciform specimen were evaluated by finite element analysis and compared to validate measured strain level and ratio. Biaxial load ratio to obtain the final biaxial failure strains with prescribed strain ratio was calculated based on the relationships between biaxial load and strain under uniaxial loadings. High speed photographs of biaxial fracture indicated that failure was initiated at gauge area and breakage was developed to GFRP tab regions in the specimen. In the first quadrant of failure strain envelope, y directional failure stains were approximately constant irrespective of xdirectional failure strain. However, fracture strains in the second quadrant of the failure envelope were larger than those in the first quadrant. Failure strains under uniaxial stress measured with the cruciform specimens were compared with those measured with the strip specimens. Approximated accordance of fracture strains under uniaxial stress
8 irrespective of specimen type indicated validity of inplane biaxial strength tests with cruciform specimens. References 1. Hinton M.J., Kaddour A.S. and Soden P.D., Failure Criteria in Fibre Reinforced Polymer Composites: The WorldWide Failure Exercise, Elsevier Science Ltd, Oxford, UK, Mailly L. and Wang S.S., Recent Development of Planar Cruciform Experiment on Biaxial Tensile Deformation and Failure of Unidirectional Glass/Epoxy Composite, Journal of Composite Materials, Vol. 42, No. 13, pp , Smits A., Van Hemelrijcka D., Philippidisb T.P. and Cardona A., Design of a Cruciform Specimen for Biaxial Testing of Fibre Reinforced Composite Laminates, Composites Science and Technology, Vol. 66, No. 78, pp , Welsh J.S., Mayes J.S. and Biskne A.C., 2D Biaxial Testing and Failure Predictions of IM7/9772 Carbon/Epoxy QuasiIsotropic Laminates, Composite Structures, Vol. 75, No. 14, pp , Susuki I., Strength Properties of Composite Laminate under Biaxial Loadings, Proceedings of the Tenth International Conference on Composite Materials (ICCM10)  Volume IV: Characterization and Ceramic Matrix Composites, pp , Khamseh A.R. and Waas A. M., Failure Mechanisms of Composite Plates with a Circular Hole under Remote Biaxial Planar Compressive Loads, Journal of engineering materials and technology, Vol. 119, No. 1, pp , Strain (%) HTA/#101 (0/90/45/45)s #02 Fx : Fy = 1 : 0 ε x (experiment) ε y (experiment) ε x (FEM) ε y (FEM) Strain (%) HTA/#101 (0/90/45/45)s #06 Fx : Fy = 1 : 1 ε x (experiment) ε y (experiment) ε x (FEM) ε y (FEM) Load Fx(kN) Load Fy (kn) (a) F x : F y = 1 : 0 (b) F x : F y = 1 : 1 Fig. 6. Comparison between measured and calculated strains under biaxial load (F x : F y =1:0 and 1:1).
9 Strain (%) HTA/#101 (0/90/45/45)s #02 Fx : Fy = 1 : 0 ε x ε y σ x σ y Stress (MPa) Load Fx(kN) Fig. 7. Biaxial strain and stress under uniaxial load (F x : F y =1:0). Table 3. Ratio of biaxial strain, load and stress. strain ratio load ratio stress ratio εx:εy F x:f y σx:σy 1:1 1:1 1:1 0.3:1 0.68:1 0.56:10.3:1 0.21:1 0.01:10.7:10.34:10.5:11:11:11: HTA/#101 (0/90/45/45)s #15 Fx : Fy = 0.21 : 1 : ε X : ε Y HTA/#101 (0/90/45/45)s #17 Fx : Fy = 1 : 1 : ε X : ε Y Strain (%) 0.5 Strain (%) Load Fy (kn) Load Fy (kn) (a) F x : F y = 0.21 : 1 (b) F x : F y = 1 : 1 Fig. 8. Loadstrain curves under biaxial loading ratio F x : F y =1:1 and 0.21:1.
10 Fig.9. High Speed photograph of fracture in gauge area of cruciform specimen under biaxial loading (F x : F y =1:1). y x (a) F x : F y = 0.21 : 1 (b) F x : F y = 1 : 1 Fig.10. Fracture of cruciform specimens under biaxial loading (F x : F y = 0.21:1 and 1:1) 2 HTA/#101quasiisotropic : cruciform specimen : strip specimen ε Y (%) ε X (%) Fig. 11. Biaxial failure strain of CF/Epoxy quasiisotropic laminates.
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationNUMERICAL MODELING OF GAS LEAKAGE THROUGH DAMAGED COMPOSITE LAMINATES
NUMERICAL MODELING OF GAS LEAKAGE THROUGH DAMAGED COMPOSITE LAMINATES Hisashi Kumazawa*, John Whitcomb** [Hisashi Kumazawa]:kumazawa.hisashi@jaxa.jp *Structure Technology Center, Japan Aerospace Exploration
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationPREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP
PREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP R. R. Pinto 1, P. P. Camanho 2 1 INEGI  Instituto de Engenharia Mecanica e Gestao Industrial, Rua Dr. Roberto Frias, 4200465, Porto, Portugal 2 DEMec,
More informationFailure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationDAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS DAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT A. Yoshimura 1*, T. Okabe, M. Yamada 3, T. Ogasawara 1, Y. Tanabe 3 1 Advanced
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationFailure Analysis of Unidirectional Composite Pinned Joints
217 IJEDR Volume, Issue 4 ISSN: 23219939 Failure Analysis of Unidirectional Composite Pinned Joints 1 Sai Ashok.M, 2 Mr. U. Koteswara Rao 1 Mtech Machine Design, 2 Associate Professor & Asst. COE 1
More informationNUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION
NUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION Fabrice PIERRON*, François CERISIER*, and Michel GRÉDIAC** * SMS/ Département Mécanique et Matériaux, École Nationale Supérieure
More informationCOMPARISON OF NUMERICAL SIMULATION AND EXPERIMENT OF A FLEXIBLE COMPOSITE CONNECTING ROD
10th International DAAAM Baltic Conference "INDUSTRIAL ENGINEERING  1213 May 2015, Tallinn, Estonia COMPARISON OF NUMERICAL SIMULATION AND EXPERIMENT OF A FLEXIBLE COMPOSITE CONNECTING ROD Sedláček,
More informationCoupling of plasticity and damage in glass fibre reinforced polymer composites
EPJ Web of Conferences 6, 48 1) DOI: 1.151/epjconf/1648 c Owned by the authors, published by EDP Sciences, 1 Coupling of plasticity and damage in glass fibre reinforced polymer composites R. Kvale Joki
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationSKINSTRINGER DEBONDING AND DELAMINATION ANALYSIS IN COMPOSITE STIFFENED SHELLS
SKINSTRINER DEBONDIN AND DELAMINATION ANALYSIS IN COMPOSITE STIFFENED SHELLS R. Rikards, K. Kalnins & O. Ozolinsh Institute of Materials and Structures, Riga Technical University, Riga 1658, Latvia ABSTRACT
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More information2 Experiment of GFRP bolt
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FATIGUE LIFE EVALUATION OF BOLT MADE OF WOVEN FABRIC FRP Takeshi INOUE*, Hiroaki NAKAI**, Tetsusei KURASHIKI**, Masaru ZAKO**, Yuji KOMETANI*** *Graduate
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationDynamic analysis of Composite Micro Air Vehicles
Dynamic analysis of Composite Micro Air Vehicles Shishir Kr. Sahu Professor and Head, Civil Engineering, National Institute of Technology, Rourkela, India Email: sksahu@nitrkl.ac.in ABSTRACT The present
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationModule 7: Micromechanics Lecture 25: Strength of Materials Approach. Introduction. The Lecture Contains. Effective Transverse Modulus
Introduction In the previous lecture we have introduced the concept of Representative Volume Element or Unit Cell. This is the basic building block in a micromechanical study. Further, we explained the
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationCOMPRESSIVE BEHAVIOR OF IMPACT DAMAGED COMPOSITE LAMINATES
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS COMPRESSIVE BEHAVIOR OF IMPACT DAMAGED COMPOSITE LAMINATES Hiroshi Suemasu*, Wataru Sasaki**, Yuuichiro Aoki***, Takashi Ishikawa**** *Department of
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More information2D biaxial testing and failure predictions of IM7/9772 carbon/epoxy quasiisotropic laminates q
Composite Structures 75 (2006) 60 66 www.elsevier.com/locate/compstruct 2D biaxial testing and failure predictions of IM7/9772 carbon/epoxy quasiisotropic laminates q Jeffry S. Welsh a, *, J. Steven
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationMultiscale Approach to Damage Analysis of Laminated Composite Structures
Multiscale Approach to Damage Analysis of Laminated Composite Structures D. Ivančević and I. Smojver Department of Aeronautical Engineering, Faculty of Mechanical Engineering and Naval Architecture, University
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationRATEDEPENDENT OFFAXIS COMPRESSIVE STRENGTH OF A UNIDIRECTIONAL CARBON/EPOXY LAMINATE AT HIGH TEMPERATURE
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS RATEDEPENDENT OFFAXIS COMPRESSIVE STRENGTH OF A UNIDIRECTIONAL CARBON/EPOXY LAMINATE AT HIGH TEMPERATURE Masamichi KAWAI *, Satoru SAITO **, JianQi
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationME 2570 MECHANICS OF MATERIALS
ME 2570 MECHANICS OF MATERIALS Chapter III. Mechanical Properties of Materials 1 Tension and Compression Test The strength of a material depends on its ability to sustain a load without undue deformation
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationNUMERICAL SIMULATION OF DAMAGE IN THERMOPLASTIC COMPOSITE MATERIALS
5 th European LSDYNA Users Conference Composites NUMERICAL SIMULATION OF DAMAGE IN THERMOPLASTIC COMPOSITE MATERIALS Kevin Brown 1, Richard Brooks, Nicholas Warrior School of Mechanical, Materials and
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationA RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION
A RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION H. Debski a*, J. Bienias b, P. Jakubczak b a Faculty of Mechanical Engineering, Department of Machine
More informationDAMAGE MECHANICS MODEL FOR OFFAXIS FATIGUE BEHAVIOR OF UNIDIRECTIONAL CARBON FIBERREINFORCED COMPOSITES AT ROOM AND HIGH TEMPERATURES
DAMAGE MECHANICS MODEL FOR OFFAXIS FATIGUE BEHAVIOR OF UNIDIRECTIONAL CARBON FIBERREINFORCED COMPOSITES AT ROOM AND HIGH TEMPERATURES M. Kawai Institute of Engineering Mechanics University of Tsukuba,
More informationEXPERIMENTAL AND THEORETICAL STUDY OF THE DAMAGE ONSET IN BIAXIAL CRUCIFORM SPECIMENS UNDER STATIC AND HYSTERESIS LOADING
EXPERIMENTAL AND THEORETICAL STUDY OF THE DAMAGE ONSET IN BIAXIAL CRUCIFORM SPECIMENS UNDER STATIC AND HYSTERESIS LOADING E. Lamkanfi a,1, C. Ramault 2, A. Makris 2, W. Van Paepegem 1, J. Degrieck 1, D.
More informationComparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost
Comparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department
More informationA STRUCTURE DESIGN OF CFRP REAR PRESSURE BULKHEAD WITHOUT STIFFENERS
Xi an, 225 th August 217 A STRUCTURE DESIGN OF CFRP REAR PRESSURE BULKHEAD WITHOUT STIFFENERS LI Zhongyang 1, LI Dong 2 Mailbox7235, Yanliang District, Xian, China, Email: zhongyangli@live.com Keywords:
More informationInfluence of fibre proportion and position on the machinability of GFRP composites An FEA model
Indian Journal of Engineering & Materials Sciences Vol. 12, October 2005, pp. 443450 Influence of fibre proportion and position on the machinability of GFRP composites An FEA model D Abdul Budan* Department
More informationSize Effects In the Crushing of Honeycomb Structures
45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference 1922 April 2004, Palm Springs, California AIAA 20041640 Size Effects In the Crushing of Honeycomb Structures Erik C.
More information[5] Stress and Strain
[5] Stress and Strain Page 1 of 34 [5] Stress and Strain [5.1] Internal Stress of Solids [5.2] Design of Simple Connections (will not be covered in class) [5.3] Deformation and Strain [5.4] Hooke s Law
More informationThe numerical simulation research of an UltraLight Photovoltaic Cell multilayer composite structure
5th International Conference on Civil, Architectural and Hydraulic Engineering (ICCAHE 2016) The numerical simulation research of an UltraLight Photovoltaic Cell multilayer composite structure Kangwen
More informationFINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Ever J. Barbero Department of Mechanical and Aerospace Engineering West Virginia University USA CRC Press Taylor &.Francis Group Boca Raton London New York
More informationTHE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS THE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES L.V. Smith 1 *, M. Salavatian 1 1 School of Mechanical and Materials
More informationKeywords: Adhesively bonded joint, laminates, CFRP, stacking sequence
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS GLOBAL AND LOCAL INFLUENCE OF STACKING SEQUENCE ON THE STRENGTH OF ADHESIVELY BONDED JOINTS OF CFRP LAMINATES J. Rousseau*, P. Satthamnuwong DRIVE,
More informationMECHANICS OF MATERIALS
CHATR Stress MCHANICS OF MATRIALS and Strain Axial Loading Stress & Strain: Axial Loading Suitability of a structure or machine may depend on the deformations in the structure as well as the stresses induced
More informationImpact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics
Impact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics Dr. A. Johnson DLR Dr. A. K. Pickett ESI GmbH EUROPAM 99 Impact and Crash Modelling of Composite Structures: A Challenge
More informationFINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE
FINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE M. Růžička, V. Kulíšek 2, J. Had, O. Prejzek Department of Mechanics, Biomechanics and Mechatronics, Faculty of Mechanical
More informationFracture Mechanics, Damage and Fatigue: Composites
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue: Composites Ludovic Noels Computational & Multiscale Mechanics of Materials CM3 http://www.ltascm3.ulg.ac.be/
More informationPREDICTION OF OPEN HOLE COMPRESSIVE FAILURE FOR QUASIISOTROPIC CFRP LAMINATES BY MMF/ATM METHOD
HE 19 H INERNAIONAL CONFERENCE ON COMPOSIE MAERIALS PREDICION OF OPEN HOLE COMPRESSIVE FAILURE FOR QUASIISOROPIC CFRP LAMINAES BY MMF/AM MEHOD. Hioki 1*, M. Nakada 2, Y. Miyano 2, H. Katoh 3 1 Graduate
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationAnalysis of nonlinear shear deformations in CFRP and GFRP textile laminates
Loughborough University Institutional Repository Analysis of nonlinear shear deformations in CFRP and GFRP textile laminates This item was submitted to Loughborough University's Institutional Repository
More informationNUMERICAL FEM ANALYSIS FOR THE PART OF COMPOSITE HELICOPTER ROTOR BLADE
Journal of KONES Powertrain and Transport, Vol. 19, No. 1 2012 NUMERICAL FEM ANALYSIS FOR THE PART OF COMPOSITE HELICOPTER ROTOR BLADE Hubert D bski Lublin University of Technology, Department of Machine
More informationUSE OF DIGITAL IMAGE CORRELATION TO OBTAIN MATERIAL MODEL PARAMETERS FOR COMPOSITES
USE OF DIGITAL IMAGE CORRELATION TO OBTAIN MATERIAL MODEL PARAMETERS FOR COMPOSITES Brian Croop, Hubert Lobo (DatapointLabs, USA). Presenter: Hubert Lobo, President SUMMARY The development of material
More informationProject MMS13 Task 5 Report No 3 (M6/D3)
Project MMS13 Task 5 Report No 3 (M6/D3) Material Data Requirements and Recommended Test Methods for the Predictive Modelling of Defect Criticality in Composite Material Systems M R L Gower and G D Sims
More informationCOMPARISON OF EXPERIMENTAL RESULTS WITH FEM ONES OF RECTANGULAR CFRP TUBES FOR FRONT SIDE MEMBERS OF AUTOMOBILES
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS COMPARISON OF EXPERIMENTAL RESULTS WITH FEM ONES OF RECTANGULAR CFRP TUBES FOR FRONT SIDE MEMBERS OF AUTOMOBILES HyoungSoo Kim*, Goichi Ben**,Yoshio
More informationStressstrain response and fracture behaviour of plain weave ceramic matrix composites under uniaxial tension, compression or shear
Xi an 225 th August 217 Stressstrain response and fracture behaviour of plain weave ceramic matrix composites under uniaxial tension compression or shear Heyin Qi 1 Mingming Chen 2 Yonghong Duan 3 Daxu
More informationCalculation of Damagedependent Directional Failure Indices from the TsaiWu Static Failure Criterion
Van Paepegem, W. and Degrieck, J. (3. alculation of Damagedependent Directional Failure Indices from the saiwu Static Failure riterion. omposites Science and echnology, 63(, 353. alculation of Damagedependent
More informationSIZE EFFECTS IN THE COMPRESSIVE CRUSHING OF HONEYCOMBS
43rd AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Con 2225 April 2002, Denver, Colorado SIZE EFFECTS IN THE COMPRESSIVE CRUSHING OF HONEYCOMBS Erik C. Mellquistand Anthony M.
More informationModeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites
Modeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites H.E.Pettermann 1, C.Schuecker 1, D.H.Pahr 2, F.G.Rammerstorfer 2 1 Austrian Aeronautics
More informationStrength of GRPlaminates with multiple fragment damages
Strength of GRPlaminates with multiple fragment damages S. Kazemahvazi, J. Kiele, D. Zenkert Kungliga Tekniska Högskolan, KTH 100 44 Stockholm, Sweden sohrabk@kth.se SUMMARY The strength of glass fibre
More informationIMPACT STRENGTH AND RESPONSE BEHAVIOR OF CFRP GUARDER BELT FOR SIDE COLLISION OF AUTOMOBILES
IMPACT STRENGTH AND RESPONSE BEHAVIOR OF CFRP GUARDER BELT FOR SIDE COLLISION OF AUTOMOBILES AOKI Y.*, BEN G.**, KIM H. S.* *College of Science & Technology, Nihon University **College of Industrial Technology,
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationFig. 1. Circular fiber and interphase between the fiber and the matrix.
Finite element unit cell model based on ABAQUS for fiber reinforced composites Tian Tang Composites Manufacturing & Simulation Center, Purdue University West Lafayette, IN 47906 1. Problem Statement In
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationUniversity of Sheffield The development of finite elements for 3D structural analysis in fire
The development of finite elements for 3D structural analysis in fire Chaoming Yu, I. W. Burgess, Z. Huang, R. J. Plank Department of Civil and Structural Engineering StiFF 05/09/2006 3D composite structures
More informationMechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces
Mechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces PingCheung Tse epartment of Mechanical Engineering, The Hong Kong Polytechnic University, Hunghom, Kowloon, Hong Kong
More informationFLEXURAL RESPONSE OF FIBER RENFORCED PLASTIC DECKS USING HIGHERORDER SHEAR DEFORMABLE PLATE THEORY
AsiaPacific Conference on FRP in Structures (APFIS 2007) S.T. Smith (ed) 2007 International Institute for FRP in Construction FLEXURAL RESPONSE OF FIBER RENFORCED PLASTIC DECKS USING HIGHERORDER SHEAR
More informationBioMechanics and BioMaterials Lab (BME 541) Experiment #5 Mechanical Prosperities of Biomaterials Tensile Test
BioMechanics and BioMaterials Lab (BME 541) Experiment #5 Mechanical Prosperities of Biomaterials Tensile Test Objectives 1. To be familiar with the material testing machine(810le4) and provide a practical
More informationSpecial edition paper
Development of New Aseismatic Structure Using Escalators Kazunori Sasaki* Atsushi Hayashi* Hajime Yoshida** Toru Masuda* Aseismatic reinforcement work is often carried out in parallel with improvement
More informationMulti Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala
Multi Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala Abstract: FRP laminated composites have been extensively used in Aerospace and allied industries
More informationKINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP)
KINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP) 1 University of Science & Technology Beijing, China, niukm@ustb.edu.cn 2 Tsinghua University, Department of Engineering Mechanics, Beijing, China,
More informationSamantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2
Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force
More informationPOSTPEAK BEHAVIOR OF FRPJACKETED REINFORCED CONCRETE COLUMNS
POSTPEAK BEHAVIOR OF FRPJACKETED REINFORCED CONCRETE COLUMNS  Technical Paper  Tidarut JIRAWATTANASOMKUL *1, Dawei ZHANG *2 and Tamon UEDA *3 ABSTRACT The objective of this study is to propose a new
More informationIJSER 1. INTRODUCTION. M.Elhadary
1591 A new failure criterion for GRP composite materials subjected to inphase and outofphase biaxial fatigue loading under different stress ratios M.Elhadary Abstract this studying the fatigue behavior
More informationStrength Prediction Of Composite Laminate
Strength Prediction Of Composite te Prof. Yogananda. A 1, Mr. R. Vijayakumar 2 Assistant Professor, Department of Mechanical Engineering, East West Institute of Technology, Bangalore. Research Scholar,
More informationInternational Journal of Innovative Research in Science, Engineering and Technology Vol. 2, Issue 7, July 2013
ANALYSIS AND MITIGATION OF STRESS CONCENTRATION FACTOR OF A RECTANGULAR ISOTROPIC AND ORTHOTROPIC PLATE WITH CENTRAL CIRCULAR HOLE SUBJECTED TO INPLANE STATIC LOADING BY DESIGN OPTIMIZATION Shubhrata Nagpal
More informationME 243. Mechanics of Solids
ME 243 Mechanics of Solids Lecture 2: Stress and Strain Ahmad Shahedi Shakil Lecturer, Dept. of Mechanical Engg, BUET Email: sshakil@me.buet.ac.bd, shakil6791@gmail.com Website: teacher.buet.ac.bd/sshakil
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationEXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS
EXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS Umar Farooq and Karl Gregory School of Built Environment and Department of Engineering, University of Bolton,
More informationMODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE
MODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE Jean Paul Charles, Christian Hochard,3, Pierre Antoine Aubourg,3 Eurocopter, 375 Marignane cedex, France Unimeca, 6 rue J. Curie, 3453
More informationFEAnalysis of Stringertofloorbeam Connections in Riveted Railway Bridges
FEAnalysis of Stringertofloorbeam Connections in Riveted Railway Bridges By Mohammad AlEmrani 1 and Robert Kliger 2 Department of Structural Engineering Chalmers University of Technology, SE412 96
More information4.MECHANICAL PROPERTIES OF MATERIALS
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stressstrain diagram
More informationIn Situ Ultrasonic NDT of Fracture and Fatigue in Composites
ECNDT 26  Mo.2.6.5 In Situ Ultrasonic NDT of Fracture and Fatigue in Composites I. SOLODOV, K. PFLEIDERER, and G. BUSSE Institute for Polymer Testing and Polymer Science (IKP), Nondestructive Testing
More informationFig. 1. Different locus of failure and crack trajectories observed in mode I testing of adhesively bonded double cantilever beam (DCB) specimens.
a). Cohesive Failure b). Interfacial Failure c). Oscillatory Failure d). Alternating Failure Fig. 1. Different locus of failure and crack trajectories observed in mode I testing of adhesively bonded double
More informationPrediction of The Ultimate Strength of Composite Laminates Under InPlane Loading Using A Probabilistic Approach
Prediction of the Ultimate Strength of Composite Laminates Under InPlane Loading Prediction of The Ultimate Strength of Composite Laminates Under InPlane Loading Using A Probabilistic Approach Tae Jin
More informationMECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING
MECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING Steven Roy, Larry Lessard Dept. of Mechanical Engineering, McGill University, Montreal, Québec, Canada ABSTRACT The design and
More informationAn orthotropic damage model for crash simulation of composites
High Performance Structures and Materials III 511 An orthotropic damage model for crash simulation of composites W. Wang 1, F. H. M. Swartjes 1 & M. D. Gan 1 BU Automotive Centre of Lightweight Structures
More informationPREDICTION OF BUCKLING AND POSTBUCKLING BEHAVIOUR OF COMPOSITE SHIP PANELS
FONDATĂ 1976 THE ANNALS OF DUNAREA DE JOS UNIVERSITY OF GALATI. FASCICLE IX. METALLURGY AND MATERIALS SCIENCE N 0. 007, ISSN 15 08X PREDICTION OF BUCKLING AND POSTBUCKLING BEHAVIOUR OF COMPOSITE SHIP PANELS
More informationStress intensity factors for an inclined and/or eccentric crack in a finite orthotropic lamina
1886 Stress intensity factors for an inclined and/or eccentric crack in a finite orthotropic lamina Abstract Stress intensity factors (SIF) are determined for an inclined and / or eccentric crack in a
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More information